- freely available
Sensors 2010, 10(4), 2638-2674; doi:10.3390/s100402638
Published: 25 March 2010
Abstract: Films of conducting polymers can be oxidized and reduced in a reversible way. Any intermediate oxidation state determines an electrochemical equilibrium. Chemical or physical variables acting on the film may modify the equilibrium potential, so that the film acts as a sensor of the variable. The working potential of polypyrrole/DBSA (Dodecylbenzenesulfonic acid) films, oxidized or reduced under constant currents, changes as a function of the working conditions: electrolyte concentration, temperature or mechanical stress. During oxidation, the reactive material is a sensor of the ambient, the consumed electrical energy being the sensing magnitude. Devices based on any of the electrochemical properties of conducting polymers must act simultaneously as sensors of the working conditions. Artificial muscles, as electrochemical actuators constituted by reactive materials, respond to the ambient conditions during actuation. In this way, they can be used as actuators, sensing the surrounding conditions during actuation. Actuating and sensing signals are simultaneously included by the same two connecting wires.
Most of the technological advances developed by humans are inspired on natural systems, organs, functions or devices present in living creatures and developed through millions of years of biological evolution. Natural systems and devices combine efficiency with intellectual, scientific and technological elegance.
Accordingly, natural muscles are elegant devices developed to transform chemical energy into mechanical energy and heat . With respect to actuation, the main difference between human technology and natural muscles is that during actuation the chemical composition changes inside the wet organ, meanwhile dry materials from artificial machines keep a constant composition. The actuation of a natural muscle (Figure 1) involves: (a) aqueous media, (b) electric pulses arriving from the brain (the pulse generator) to the muscle through the nervous system, (c) liberation of calcium ions inside the sarcomere, (d) chemical reactions, (e) conformational changes along natural polymeric chains (actin and myosin) with change of the sarcomere volume and (f) water interchange. This natural motor is able to perform elegant and gentle movements still not reproduced by any man-made motor. Moreover, the actuation of the muscle involves simultaneous sensing processes, providing living creatures with a perfect consciousness of characteristics of the mechanical movements and physical interactions between the organ moved by the muscle and its environment.
The chemical and physical processes linked to the electrochemistry of conducting polymers present a great deal of similarities with the above described biological processes, much more similar than those linked to any other artificial material [2–6].
2. Conducting Polymers: Classification
Substituted polymers [27,29–31]. One, or several, hydrogen atoms from the basic monomer was replaced by another chemical group. Hundreds of different chemical groups can be used to obtain new substituted monomers and polymers.
Polymer/macro-ion blends. The synthesized oxidized material contains macro-ions, which are not interchanged during redox processes:
Every component of a family originates, by electrochemical oxidation or reduction, hundreds of oxidized materials (polymer/counterion/solvent), depending on the salt used in the solution during the electrochemical reaction.
3. Electrochemical Behavior of Conducting Polymers in Solution
During electrochemical oxidation (or reduction) of neutral polymeric chains, positive (or negative) charges are stored along the polymeric chains (Figure 3) and balancing counterions are forced to penetrate from the solution [2–6,51,52] to generate a new material (polyelectrolyte).
Depending on the balancing ion, different materials (polyeletrolytes) are obtained. The emerging positive (or negative) charges on the chains induce strong polymer/solvent interactions forcing the entrance of solvent from the solution. A complex material, polymer/ion/solvent is obtained.
There exist two kinds of oxidation processes:
Where s means solid and sol is solution, MA− represents any charge balancing macro-anions trapped inside the CP during polymerization, pPy represent the polypyrrole (or any other CP) chains and C+ represent a cation. The role of the solvent molecules in this case is not clear, due to the permanent presence of ionic species in the material interacting with the solvent dipolar moment. Reactions (1) and (2) produce positive charges on the polymeric chains: those processes are also named ‘p- doping’.
Some conducting polymers, as most of the polythiophene families, can also be reduced and reoxidized from the neutral state, storing negative charges (‘n-doping’) along the chains at high cathodic potential (stable electrolytes are required) interchanging balancing cations [59,60]:
In general, two basic redox processes can occur from CPs:
All of the above-described reactions are simplified versions. Any film of a conducting polymer establishes a physical equilibrium between solvent, anions and cations in the polymer matrix and in the electrolyte. So the charge balance is determined by simultaneous interchange of anions, cations and solvent across the polymer/solvent interface [61–64]. For each family one of the reactions (1) or (2) prevails. The final result of reactions (1), (2), or (3) is a polymeric salt, a polyelectrolyte.
4. Electrochemical Properties
Any of those electrochemical reactions promotes a continuous movement of anions or cations across the film/solution interface. The obtained polymeric salts are non-stoichiometric compounds [65,66]. The three considered reactions are reversible, so the stoichiometry of the material can be adjusted to any intermediate content between non-charged (reduced) polymer and fully oxidized polymer (around 50% of counterion content). Some properties change as a function of the material composition: conductivity, electro-chemo-mechanical effects (change of volume), electrochromic properties, charge storage, chemical storage and electroporosity [2–6,51,52]. These are described as follows:
- Electrochemo-mechanical properties: the entrance and expulsion of counterions and solvent from the solution, driven by the electrochemical reaction, promotes reversible changes on the material volume, (see Figure 4), which can be applied to generate macroscopic movement and mechanical energy [67–70].
- Electrochromic properties: the reversible reorganization of the double bonds along the polymeric chains generates and destroys chromophores (polarons and bipolarons) adsorbing light along the UV-vis and near IR regions of the spectra. The color of the material can be changed reversibly, by controlling the concentration of chromophores, under electrochemical reaction in a continuous and reversible manner [71–75].
- Charge storage: transition from neutral to oxidized polymers implies the storage of positive charges along the polymeric chains. Transition from neutral to reduced polymer implies the storage of negative charges along the polymeric chains. Therefore, CPs can be used as electrodic materials for polymeric batteries [76–78].
- Porosity: a film of a basic conducting polymer in a neutral state is a porous compacted structure, in which average distances between chains is short. During oxidation, coulombic repulsions among the emerging positive charges in neighboring chains increase the average distance between chains allowing counterions entrance [54,79–81].
- Electron/Chemical transduction: reverse electrochemical reactions are linked to the simultaneous interchange of chemical ions between the CP and the solution. This must be a univoque relationship; each injected electron forces the interchange of an one-valence chemical ion with the ambient electrolyte, suitable for a reversible storage and release of chemical and pharmacological compounds [82–84].
5. Multifunctional and Biomimicking Properties
The above described properties are linked to any of the electrochemical reactions: (1), (2) or (3), taking place in soft and wet materials, with a composition resembling that of animal organs: solvent, ions and polymeric (organic) molecules. Every property is linked to one or several similar functions occurring in biological organs [3,5,85–89], as shown in Table 1.
The electrochemical oxidation/reduction of any non-stoichiometric CP produces a multifunctional actuation of biomimetic properties. Only one reaction generates multiple properties.
6. Unparalleled Simultaneous Sensing Possibilities
The reverse electrochemical processes, (1), (2) or (3), suppose that any intermediate composition of the material is linked to an electrochemical equilibrium between: polymeric species, counterions and solvent inside the polymer; ions and solvent in solution, and electrons in the metal:
That means that any physical variable, such as mechanical (through ΔV), optical (through [pPyn+], polaronic and bipolaronic chromophores), electrical (applied i or E), magnetic (through [pPyn+], as radical-cations), etc., or chemical variable, such as counterion concentration [A−]aq, ionic strength (I), or temperature (through the kinetic coefficient), acting on the electrochemical equilibrium, must promote a simultaneous energetic change of the electrons in the metal, which can be detected by means of a potentiostat. Working under equilibrium conditions the simplified expression of the Nerst equation as a function of the concentrations can be applied:
The sensing concept works under equilibrium, and under transition conditions. If we consider a single, lineal and ideal chain of conducting polymer (CP) constituted by m monomeric units, the reaction goes, through n consecutive oxidation equilibrium steps (m > n):
The reaction goes on through n consecutive energetic conformational (electronic) states of the polymeric chain, with increasing conjugated planar segments. Each of those conformational electronic states establishes a fast electronic equilibrium, due to the high conductivity of the material, with electrons in the connecting metal. So, under transition conditions the electrode potential reflects the average conformational electronic state of the chains in the reacting film at any time during the reaction.
Both aspects, the slow chemical equilibrium and the fast electronic equilibrium, include the influence of all the above (reaction 5) chemical and physical variables on the electrode potential both, under equilibrium, or along the reaction. Consequently, any possible devices constructed on the bases of the described electrochemical properties are expected to work, simultaneously, as sensors of the ambient conditions [90–93]. Any of those devices should sense the ambient, while working, as the natural organs do, overcoming any unprecedented device that requires separate actuating and sensing systems with separate electrical connections.
The simultaneous actuating/sensing abilities of any electrochemical device based on conducting polymers (or similar organic materials as fullerenes, carbon nanotubes, graphenes,…) must be related to the sensing abilities of the self-supported material films under electrochemical reactions. This behavior will be illustrated for thick polypyrrole/DBSA films.
7. Film preparation of Polypyrrole in Dodecyl Benzene Sulfonate (DBSA) Aqueous Solutions
Polypyrrole films were prepared at room temperature (20 ± 2 °C) in dark conditions in a one-compartment electrochemical cell from an aqueous solution of 0.2 M DBSA and 0.2 M pyrrole. The working electrode was an AISI 316 stainless steel sheet, having a surface area of 5 cm2 on either side. Deposition was performed on both sides of the electrode. Two larger electrodes (10 cm2) of the same material were used as counter electrodes, placed symmetrically on both sides of the working electrode in order to obtain a uniform electrical field. A standard Ag/AgCl electrode from Metrohm was used as reference electrode.
Polypyrrole (pPy) was electrogenerated by applying a constant anodic current density of 2 mA cm−2 during two hours. The overall charge consumed during the electropolymerization was 72.0 C. Two separate films were obtained, coating each of the electrode faces, with a mass of 32 ± 0.2 mg each, determined by means of a precision balance (±0.1 μg) by weight differences between coated and uncoated electrodes. After peeling from the working electrode, the films were submerged in de-ionized water for 24 hours to remove DBSA excess from the polymer surface. Film thicknesses of 85 ± 10 μm were measured using a COMECTA electronic digital micrometer with a precision of ±1 μm. All electrochemical studies were performed using an Autolab PGSTAT-100 potentiostat/galvanostat controlled by a personal computer using GPES electrochemical software. The electrochemical measurements were carried out in 0.1 M LiClO4 aqueous solutions, using the self-supported polymer film as the working electrode, a stainless steel counterelectrode and an Ag/AgCl reference electrode (Figure 5a). A Julabo T25 Cryostat/Thermostat (±0.1 °C) was used to study the influence of the temperature. All the other experiments were performed at 20 °C (room temperature).
7.1. Voltammetric Response
Figure 5b shows the experimental voltammogram recorded between +0.8 V, as anodic potential limit and −2.0 V, as cathodic potential limit, with 6 mV·s−1 the scan rate. Only one cathodic maximum, at −0.850 V, and one anodic maximum, at 0.356 V, are observed. The shape of the obtained voltammogram and peak potentials are similar to those reported for thinner pPy/DBS films [94–96] in aqueous solutions and quite different to those reported for pPy/ClO4− films . Here a larger potential separation between anodic and cathodic peaks is observed, which can be attributed to use of a thicker film. These results indicate that dodecyl benzene sulfonate (DBS−) is the prevailing counterion inside the material. Due to its large size, the counterion remains trapped, promoting an exchange of Li+ cations predominately during oxidation/reduction processes. This interchange will promote the insertion of cations and polymeric swelling during reduction and the cations expulsion with polymeric shrinking during oxidation. These volume changes were confirmed by the sense of the angular movements of a pPy/tape actuator under the flow of anodic and cathodic currents.
The electrochemical reaction can be written in a simplified form as:
The reaction occurring from left to right is the anodic process in which electrons are extracted from the polymeric chains. In Figure 5b, this process occurs during the anodic currents giving the maximum at 0.356 V. The charge extracted during oxidation can be obtained by integration of the maximum. The reaction from the right side towards the left side is the cathodic process, that is, electrons are introduced into the polymeric chains eliminating positive charges. This process is related to the cathodic currents originating the maximum at −0.850 V (negative currents on the voltammogram). The charge injected during reduction can be obtained by integration of this maximum.
7.2. Sensing Abilities under Constant Current
In order to study the response of the material to different experimental variables, a galvanostatic procedure (Figure 6) was designed.
After stabilization of the initial oxidation state by applying a constant current of −0.150 mA for 250 s, the material film was submitted to three consecutive square waves of current (Figure 6a). The chronopotentiometric responses obtained during consecutive oxidation/reduction processes were recorded (Figure 6b).
The pPy/DBS film was submitted to different square waves of current ranging from ±1.5 to ±24 mA, passing a constant charge of ±180 mC. Figure 7 shows the obtained anodic chronopotentiograms. The potential evolves at higher potentials for higher currents. The higher initial step of the potential for rising currents is related to the different resistances present in the system: film resistance, interface resistance due to ions interchange, solution resistance and reaction resistance. After this initial change, the potential increases for rising anodic currents following the electrode processes. The electrical energy (Ee) consumed by the polymer film during each oxidation/reduction was calculated as Ee = i·∫E·dt, with i the constant current, E the electrodic potential at any time, t, of the current flow. Figure 7b shows the variation of the electrical energy as a function of the applied current. A linear fit was obtained for both cathodic and anodic processes: the material under reaction senses the applied current.
7.3. Temperature Sensor
In reaction (1) or (2), as for any other chemical or electrochemical process, the reaction rate (anodic or cathodic) is expected to increase for rising experimental temperatures, due to the Arrhenius dependence of the reaction kinetic coefficient with T. This is equivalent to saying that working at a constant reaction rate, under flow of a constant current; the reaction is expected to occur with a lower reaction resistance (that means lower potentials) for increasing temperatures. In order to gain more knowledge into the sensing abilities of the electroactive material, the film is submitted to square current waves (±4 mA for 60 s every current) at different temperatures (15, 20, 25, 30, 35 and 40 °C). Figure 8a shows the obtained chronopotentiograms in which the evolutions of the reactive film potential for the different temperatures were overlapped. Figure 8b shows the response for the last oxidation step referred to the same arbitrary zero initial potential, in order to obtain the consumed electrical energies by integration of the curves. As expected, for the anodic processes decreasing potentials are observed for the same times of current flow and increasing temperatures. Rising available thermal energies require lower consumption of electrical energies during the reaction. Under constant current this produces lower potentials. Figure 9 shows the linear increase of the consumed electrical energy for decreasing working temperatures . As a partial conclusion the electroactivity of the material, understood as electrochemical reactions of polymeric oxidation or reduction, act as a temperature sensor.
7.4. Concentration Sensor
Similar experiments were performed by changing the electrolyte concentration (0.01, 0.02, 0.05, 0.1, 0.25, 0.5 and 1 M) as shown in Figure 10. For the same time of a constant current flow, decreasing electrode potentials are observed for rising electrolyte concentrations. The effect increases when referred to the same arbitrary zero initial potential. The consumed specific electrical energy changes as a function of the concentration. (Figure 10b) We conclude that the material works as a sensor of the salt concentration in the ambient.
As final conclusions, we can state that the specific energy consumed during oxidation or reduction reactions of the studied film sense the influence of the variables: flowing current, working temperature or electrolyte concentration, on the system. The consumed electrical energy is a linear function of the studied variable.
7.5. Expected Sensing Electrochemical Devices
Those facts described in Sections 7.2 to 7.4 suggest that any device based on an electrochemical property (on the electrochemical reactions) of intrinsically conducting polymers is expected to act simultaneously as a sensor of any ambient and working variables acting on the reaction. Artificial muscles, polymeric batteries, smart membranes, drug delivery devices, electrochromic devices, among others, are expected to wear those simultaneous sensing-actuating properties. The two connecting wires should include both, actuating (i.e., the current) and sensing (i.e., the potential evolution) signals. We will focus our attention here on the present state of the art for those simultaneous actuating/sensing abilities of conducting polymers as reactive materials when used to construct artificial muscles.
8. Muscles and Artificial Muscles
Muscles are efficient devices working at constant temperature to transform chemical energy from glucose, into mechanical energy and heat. The fact that they work under constant temperature, far away from the servitude imposed by the Carnot’s principle, makes natural muscles much more efficient than any parallel human-made machine. Moreover, internal combustion devices, steam engines or turbo-reactors produce quite rudimentary movements, noise (acoustic and electromagnetic) and ambient deterioration, even though very useful for human development [98–100].
The actuation of any natural muscle is based on molecular motors constituted by polymeric chains of actin and myosin. The basic structure for the actuation is the sarcomere, where actin and myosin chains are organized as quasi-longitudinal fibers perpendicular to the sarcomere walls. The actuation mechanism of those electro-chemo-mechanical devices was described above.
8.1. Artificial Muscles
In order to mimic natural molecular motors, we shall attempt to include, at least, electric pulses and polymeric chains. Some pioneering devices were constructed in the 1950s using films of polymeric gels immersed in aqueous solutions [101–104]. At the beginning of the 1990s, a fast development of devices based on the interaction between electric fields, or electric currents, and polymers took place stimulated by the interest to reproduce commercial piezoelectric or electrostrictive (electromechanical) devices developed with inorganic materials, but using now similar properties from polymeric materials. The beginning of this explosive interest overlapped the discovery of intrinsically conductive polymers and the reverse electrochemical variation of their volume (Figure 4). This controlled volume variation envisaged the construction of new electrochemo-mechanical devices [67,105–107].
8.2. Classification of the Polymeric Artificial Muscles
Any developed device based on the interaction between electricity and polymers uses to be named artificial muscle. We can summarize the present state of the named artificial muscles, which actuation involves polymers, electric fields or electric currents, by their classification in two main areas:
- Electromechanical actuators: Artificial muscles responding mainly to electric fields, E (V), being the dimensions variation of the electroactive polymer proportional to:
E2: Electrostrictive actuators
E: Piezoelectric actuators
Electrokinetic actuators (electroosmotic)
- Electrochemomechanical devices: Artificial muscles responding mainly to electric charges, Q (mC), being the dimensions variation under control of the electrochemical reaction, and proportional to:
Q: Electrochemical actuators
Conventionally electromechanical devices have been manufactured as bending thin films of dry polymer (named electroactive material), both sides coated with a very thin metallic film required to apply the electric field. Any actuator has a triple layer structure: metal/polymer/metal (Figure 11). Linear devices from materials having a large dimension’s change with the electric field are also constructed.
Bending electrochemomechanical actuators can be manufactured as bilayers, using a metallic electrode as counterelectode to allow the current flow, or as three-layers (see below), including working and counterelectrode. In the three-layers structure, the two external films are electroactive (react electrochemically, changing volume) during current flow. The internal film is an adherent, flexible and non-conducting (or ionic conductor) polymeric film.
In the case of linear devices, they can be made of fibers of conducting polymers [108–112], or by electropolymerization of a conducting polymer on springs of helical metallic wires until the generation of a tube, or on zigzag metal wires to generate films [110,113–117]. Bundles of films or fibers are checked to produce lineal displacements of weights . Origami structures form films also provide good linear movements . Different models have been proposed to describe mechanical behavior or electro-chemomechanical deformations [120–122] of this kind of devices.
8.3. Electrochemomechanical Muscles: Volume Variation
Artificial muscles have been developed from films of CP involving electrochemical reactions (1) or (2) as origin of the volume variations. When the interchange of anion prevails (accepted for families a, b, d, e and g) during the redox processes, the volume of the film swells during oxidation and shrinks during reduction. Under prevailing cation interchange (accepted for families c and e), the material shrinks during oxidation and swells during reduction. The important role played by the solvent interchange in both oxidized and reduced materials, is an unsolved point. Dimensional changes parallel to electrochemical reactions, have been followed by different methodologies, or estimated from experimental densities and weights of dried oxidized or reduced films from the pioneering works of the electrochemistry of conducting polymers [123,124]. Those changes were confirmed at microscopic level by “in situ” AFM [125–127], ellipsometry , conductivity  measurements, in situ electrogravimetry [129,130] and others [131,132].
8.4. Electrochemical Basic Molecular Motors and Muscle Similitude
We can imagine an ideal and lineal and neutral polymeric chain connected to a metallic electrode and immersed in an electrolyte (see Figure 12). The strong intramolecular interactions originate a coil compact structure of the chain (Figure 12a). Under oxidation changes on the double bonds distribution and storage of positive charges originate conformational movements until a stick-like structure (Figure 12b). This basic molecular actuator [133,134] working in a reversible way driven by electrochemical reactions includes: electric pulses, ions and solvent interchanges between the polymer and the solution, chemical reactions, stimulation of the conformational movements along polymeric chains and changes in the inter- and intramolecular interactions. Those processes occurring in soft and wet materials mimic, at molecular level, the consecutive events involved on the actuation of a natural anisotropic muscle. At the moment it is not known how to construct artificial sarcomere like structures (brushes) with chains of conducting polymers between two metallic (or electronically conducting) films. Only three-dimensional isotropic, microscopic and stable changes of volume are available with films of conducting polymers under electrochemical reactions.
8.5. Devices Giving Macroscopic Movements
Bilayer structures of conducting polymer (CP) film/adherent polymer film [67,106,107,135,136], CP/metal [137–139], CP/solid state electrolyte , CP/CP [141,142], CP/plastic , CP/paper or CP/thin film of any flexible material metal coated (i.e., by sputtering)  have been elegant solutions to translate the microscopic changes of volume taking place in films of CP into increasing anisotropic mechanical stress gradient across the bilayer interface, generating an uniform macroscopic bending movements (Figure 13a). The presence of a metallic counterelectrode is required to allow the current flow, originating the electrochemical reaction that produces the bending movement. However, an important fraction of the consumed electrical energy is wasted to produce the electrochemical reactions occurring at the counterelectrode (such as solvent dissociation, which requires a high overpotential). Moreover those reactions will generate new chemicals and pH variations, migrating until the muscle and promoting the progressive deterioration of the actuating film.
The construction of a triple layer CP/tape/CP  allows a more efficient actuation by using the same current two times to produce opposite volume changes and avoiding the use of metallic counterelectrodes (Figure 11). One of the CP films, the working electrode (WE) acts as the anode, swells (for preferential anionic interchange during the reaction) and pushes the device. The second CP film is the counterelectrode (CE) acts as the cathode shrinks and trails the device. The CE uses to be short-circuited with the reference electrode (RE) output of the potentiostat. On this way we follow the instantaneous potential difference between the two CP films: the muscle potential. The muscle potential evolution under flow of a constant current is a result of the two electrochemical reactions: oxidation at the anode and reduction at the cathode. Consequently we expect those actuating reactions to be influenced by the ambient variables, becoming a sensor of those variables.
The three layers muscles can work outside the liquid electrolytic media using an ionic conducting membrane separating the two films of CP. This membrane can be obtained by solvent evaporation and UV irradiation [72,145,146], or by formation of interpenetrated networks [147–152]: the two films of CP are generated by chemical polymerization on the external part of the membrane film.
Different structures can be produced by combination of several double or triple layers to transform bending into linear movements, each of those structures including WE, CE and reference electrode [153–155].
The actuating films of CP can be generated by electropolymerization. Electrogeneration is compatible with micro and nanotechnologies  giving elegant and imaginative microdevices and microtools constituted by bending bilayers [69,137–139,158–165] or trilayers .
8.6. Electrochemical Nature of the Movement
Volume changes per unit of time, and the produced macroscopic movement, are expected (Equation 1) to be under control of the driving current. The Faraday’s expression should quantify the amount of interchanged ions. For driving current ranging from 8–35 mA, Figure 14a shows the experimental linear relationship between the driving current and the produced angular movement rate:
Whatever the applied current, the experimental slope is a constant, as expected for an electrochemically driven motor. Moreover, the experimental charge consumed to perform an angular movement of one degree is constant (Figure 14c) due to the overlapping evolution of the described angle as a function of the consumed charge for different driven constant currents:
Consequently, whatever the testing current the same charge is consumed in order to perform the same angular movement (Figure 14b). Equation 10 is a translation of the Faradays laws to bending electro-chemo-mechanical artificial muscles. The charge quantifies the amount of counterions interchanged, so the composition variation, the volume variation of the CP film and the stress gradient at the interface between the polymer films.
The expressions (9) and (10) can be applied to bilayers, triple-layers or complex structures [91,92,167–169]. Figure 14 quantifies the electrochemical nature of the movement. For any specific muscle, we can define the charge required to describe an angular movement of one degree (a mC degree−1). From a, the charge Q required to attain any new position (any new angle) from the actual position can be obtained:
This is an electrochemo-positioning device. Once defined the charge, Q, required to describe a defined angle, e.g., 90 degrees, the time consumed for the movement is under control of the charge flowing through the device per unit of time: the current [2,168].
The electrochemical nature of the device allows to state that different artificial muscles, having different surface area or constructed with pPy films having different film thickness (i.e., weight), must produce the same angular movement rate under variation of the same composition gradient, by flow of analogous charge per unit of time (current) and per unit of CP weight (same variation of the oxidation deep) as confirmed by Figure 15.
Allowing a more general expression than equation 9:where Ω is the angular rate (rad·s−1), i is the constant current (mA) flowing though the muscle and w is the weight of the conducting polymer films. Considering j as mC·s−1·mg−1 this expression states that the angular movement, Ω, of any artificial muscle constituted by conducting polymers is under control of the amount of charge flowing through the muscle per second and per weigh unit of the material. This j quantifies the variation of the oxidation rate (counterion’s composition change) per weight unit. As conclusion the angular movement for those artificial muscles is under control of the oxidation rate per unit of weight, as corresponds to any electrochemical device.
Thus, the electrochemical nature of the movement allows an excellent control of both the movement rate (by the applied current) and the angular position (by the charge). This means that we have a perfect electrical machine able to transform the electrical energy into mechanical energy. The electrochemically stimulated conformational movements of the polymeric chains and the concomitant changes of volume are used as transducers from the electrical energy to the mechanical energy.
8.7. Sensing Muscles
Based on the electrochemical nature of the movement, it should be expected that any mechanical, electrical, optical, thermal, magnetic or chemical variable acting on the reaction must influence the potential evolution of the working device. This should be a specific application to artificial muscles of the above described sensing abilities of the reactive material. Rising values of those variables increasing the reaction rate (electrolyte concentration or temperature) will promote an evolution of the muscle potential while moving along the same angle at lower values of the potential for the same time of current flow (Figure 16). Those variables which increase will decrease the reaction rate (mechanical stress) will promote a shift of the potential evolution while moving at higher muscle potentials [90–92,155,167–171]. Both, the muscle potential at a defined time of current flow, and the consumed electrical energy (i∫E dt) change linearly as a function of the different variables. (see Figure 17). Figures 16d and 17d indicate how the working muscle sense the different weights of steel plates adhered to the bottom of the muscle and trailed during the angular movement.
8.8. Tactile Muscles
The mechanical sensing characteristics (increase of the muscle potential when the trailed weight rises) announce the possibility to develop a tactile sensor. If an obstacle is located in the muscle’s pathway (Figure 18), before reaching the obstacle the muscle moves freely, under constant current: the evolution of the muscle potential overlaps that of the free muscle. When the muscle touches the obstacle, the mechanical resistance influences the anodic and cathodic electrochemical reactions occurring in the two constituent, anode and cathode, polymeric films. Consequently a step is observed on the muscle potential at the contact time, the potential step is proportional to the opposed mechanical resistance. Rising weights of the obstacle produce increasing potential steps (Figure 19). Both, potential step and consumed electrical energy after contact and during shifting times, follow a linear evolution as a function of the obstacle weight [172–174]. When the muscle is not able to shift the obstacle the potential steps by several volts. During actuation the muscle potential of the free muscle evolves from a few mV to hundred of mV. The muscle potential gradient at the contact time with the obstacle ranges from a few mV to several V. Actuating and sensing signals are of the same order of magnitude.
These results announce the development of a class of tools and robots where the electrical machines (actuators) are at the same time, and through the same two connecting wires, sensors of the working conditions and of the ambient variables. In contrast to conventional technologies, where actuators and sensors are independent tools, requiring different electrical connections, complexes interfaces with computers and complexes software to develop intelligent machines.
9. Limitations and Challenges
The field of electrochemomechanical actuators is an emerging field for reactive, soft, wet, non-stoichiometric (giant), multifunctional and biomimicking materials. Electrochemical properties and devices show unprecedented simultaneous actuating and sensing abilities. At short term different sensing devices can be constructed, such as: full polymeric batteries sensing the state of charge, the working temperature and the number of remaining living cycles and including ambient friend salts; smart electrochromic devices (windows, goggles, mirrors, etc.) sensing the transmission state, the working temperature, the remaining lifetime and the supported mechanical stresses; and smart membranes, or artificial glands for medical or agricultural dosage, or nervous interfaces able to sense different actuating and ambient conditions of work.
There exists some limiting conditions for a fast development of those new devices. The required theoretical models able to integrate Electrochemistry, Polymer Science, Mechanics and Thermodynamics, describing experimental results and predicting new results are starting to emerge. There exists a limited control of the polymerization processes (chemical or electrochemical) to produce tailor-made materials: the polymerization process coexists with degradation and cross-linking processes. The relative weight of the parallel reactions still has not been quantified.
Moreover, different experimental difficulties must be overcome. A triple layer muscle is at the same time a battery, but the electrical energy stored in a triple-layer muscle under actuation still cannot be recovered during the opposite movement.
But difficulties also mean opportunities. A new world of soft and wet, sensing and tactile (conscious) actuating biomimicking machines is a challenge for the intellectual energy and engineering ability of young scientists in the new emerging technological world.
Authors acknowledge financial support from Spanish Government (MCI) Project MAT2008-06702, Seneca Foundation Project 08684/PI/08, Consejería de Educación de Murcia, Plan Regional de Ciencia y Tecnología 2007–2010, Mexico Government Project UAEM-PROMEP 103.5/06/1975 and Conacyt (Mexico) Project 47066. J.A.P. also thanks Ministerio de Ciencia e Innovación of Spain for a Juan de la Cierva grant.
References and Notes
- Stryer, L.; Berg, J.M.; Tymoczko, J.L. Biochemistry, 4th ed. ed.; W.H. Freeman & Company: New York, NY, USA, 1995.
- Otero, T.F.; Rodriguez, J. Electrochemomechanical and electrochemopositioning devices: artifcial muscles. In Intrinsically Conducting Polymers: An Emerging Technology; Aldissi, M., Ed.; Kluwer: Dordrecht, The Netherlands, 1993; pp. 179–190.
- Otero, T.F. Conducting polymers, electrochemistry, and biomimicking processes. In Modern Aspects of Electrochemistry; Bockris, J.O.M., White, R.E., Conway, B.E., Eds.; Kluwer Academic/Plenum Publisher: New York, NY, USA, 1999; pp. 307–434.
- Otero, T.F. Electrochemomechanical devices based on conducting polymers. In Polymer Sensors and Actuators; de Rossi, D., Osada, Y., Eds.; Springer: Berlin, Germany, 2000; pp. 295–323.
- Otero, T.F. Biomimicking materials with smart polymers. In Structural Biological Materials. Design and Structure-Properties Relationships; Elices, M., Cahn, R.W., Eds.; Pergamon Materials Series: Amsterdam, the Netherlands, 2000; pp. 187–220.
- Otero, T.F. Artificial muscles, sensing and multifunctionality. In Intelligent Materials; Shahinpoor, M., Schenider, H.-J., Eds.; Royal Society of Chemistry: Cambridge, UK, 2008; pp. 142–190.
- Dallolio, A.; Dascola, G.; Varacca, V.; Bocchi, V. Electronic paramagnetic resonance and conductivity of a black electrolytic oxypyrrole. Cr. Acad. Sci. C. Chim 1968, 267, 433.
- Diaz, A.F.; Kanazawa, K.K.; Gardini, G.P. Electrochemical polymerization of pyrrole. J. Chem. Soc. Chem. Commun 1979, 14, 635–636.
- Diaz, A.F.; Lee, W.Y.; Logan, A.; Green, D.C. Chemical modification of a polypyrrole electrode surface. J. Electroanal. Chem 1980, 108, 377–380, doi:10.1016/S0022-0728(80)80348-2.
- Salmon, M.; Kanazawa, K.K.; Diaz, A.F.; Krounbi, M. A Chemical route to pyrrole polymer-films. J. Polym. Sci. Part C: Polym. Lett 1982, 20, 187–193, doi:10.1002/pol.1982.130200308.
- Rapi, S.; Bocchi, V.; Gardini, G.P. Conducting polypyrrole by chemical synthesis in water. Synth. Met 1988, 24, 217–221, doi:10.1016/0379-6779(88)90259-7.
- Rodriguez, J.; Grande, H.J.; Otero, T.F. Polypyrroles: from basic research to technological applications. In Handbook of Organic Conductive Molecules and Polymers; Nalwa, H.S., Ed.; John Wiley & Sons: Chichester, UK, 1997; pp. 415–468.
- Wallace, G.G.; Spinks, G.M.; Kane-Maguire, L.A.P.; Teasdale, P.R. Assembly of polypyrroles. In Conductive Electroactive Polymers: Intelligent Materials Systems; CRC Press: Boca Raton, FL, USA, 2003; pp. 51–88.
- Huang, W.S.; Humphrey, B.D.; MacDiarmid, A.G. Polyaniline, A Novel conducting polymer—morphology and chemistry of its oxidation and reduction in aqueous-electrolytes. J. Chem. Soc. Faraday Trans. I 1986, 82, 2385–2400, doi:10.1039/f19868202385.
- Letheby, H. XXIX. On the production of a blue substance by the electrolysis of sulphate of aniline. J. Chem. Soc 1862, 15, 161–163, doi:10.1039/js8621500161.
- Mohilner, D.M.; Argersinger, W.J.; Adams, R.N. Investigation of kinetics and mechanism of anodic oxidation of aniline in aqueous sulfuric acid solution at a platinum electrode. J. Am. Chem. Soc 1962, 84, 3618–3622, doi:10.1021/ja00878a003.
- Kitani, A.; Kaya, M.; Sasaki, K. Performance study of aqueous polyaniline batteries. J. Electrochem. Soc 1986, 133, 1069–1073, doi:10.1149/1.2108787.
- Trivedi, D.C. Polyanilines. In Handbook of Organic Conductive Molecules and Polymers, 2nd ed.; Nalwa, H.S., Ed.; John Wiley & Sons: Chichester, UK, 1997; pp. 505–572.
- Wallace, G.G.; Spinks, G.M.; Kane-Maguire, L.A.P.; Teasdale, P.R. Synthesis of polyanilines. In Conductive Electroactive Polymers: Intelligent Materials Systems; CRC Press: Boca Raton, FL, USA, 2003; pp. 121–160.
- Hotta, S.; Soga, M.; Sonoda, N. Novel organosynthetic routes to polythiophene and its derivatives. Synth. Met 1988, 26, 267–279, doi:10.1016/0379-6779(88)90243-3.
- Yamamoto, T.; Sanechika, K.; Yamamoto, A. Preparation of thermostable and electric-conducting poly(2,5-thienylene). J. Polym. Sci. Polym. Lett. Ed 1980, 18, 9–12, doi:10.1002/pol.1980.130180103.
- Diaz, A.F.; Crowley, J.; Bargon, J.; Gardini, G.P.; Torrance, J. B. Electrooxidation of aromatic oligomers and conducting polymers. J. Electroanal. Chem 1981, 121, 355–361, doi:10.1016/S0022-0728(81)80592-X.
- Wallace, G.G.; Spinks, G.M.; Kane-Maguire, L.A.P.; Teasdale, P.R. Synthesis and properties of polythiophenes. In Conductive Electroactive Polymers: Intelligent Materials Systems; CRC Press: Boca Raton, FL, USA, 2003; pp. 179–206.
- Tourillon, G.; Garnier, F. New electrochemically generated organic conducting polymers. J. Electroanal. Chem 1982, 135, 173–178, doi:10.1016/0022-0728(82)90015-8.
- Ohsawa, T.; Kaneto, K.; Yoshino, K. Electrical and optical-properties of electrochemically prepared polyfuran. Jpn. J. Appl. Phys 1984, 23, L663–L665, doi:10.1143/JJAP.23.L663.
- Zotti, G.; Schiavon, G.; Comisso, N.; Berlin, A.; Pagani, G. Electrochemical synthesis and characterization of polyconjugated polyfuran. Synth. Met 1990, 36, 337–351, doi:10.1016/0379-6779(90)90258-M.
- Waltman, R.J.; Diaz, A.F.; Bargon, J. Substituent effects in the electropolymerization of aromatic heterocyclic-compounds. J. Phys. Chem 1984, 88, 4343–4346, doi:10.1021/j150663a030.
- Pandey, P.C. A new conducting polymer-coated glucose sensor. J. Chem. Soc. Faraday Trans. I 1988, 84, 2259–2265, doi:10.1039/f19888402259.
- Diaz, A.F.; Castillo, J.; Kanazawa, K.K.; Logan, J.A.; Salmon, M.; Fajardo, O. Conducting poly-n-alkylpyrrole polymer-films. J. Electroanal. Chem 1982, 133, 233–239, doi:10.1016/0368-1874(82)85140-X.
- Macinnes, D.; Funt, B. L. Poly-ortho-methoxyaniline—a new soluble conducting polymer. Synth. Met 1988, 25, 235–242, doi:10.1016/0379-6779(88)90248-2.
- Somanathan, N.; Radhakrishnan, S. Optical properties of functionalized polythiophenes. Int. J. Mod. Phys. B 2005, 19, 4645–4676, doi:10.1142/S0217979205032930.
- Abdou, M.S.A.; Holdcroft, S. Self-doped conductive polymers. In Handbook of Organic Conductive Molecules and Polymers, 2nd ed.; Nalwa, H.S., Ed.; John Wiley & Sons: Chichester, UK, 1997; pp. 833–858.
- Freund, M.S.; Deore, B.A. Self-Doped Conducting Polymers; John Wiley & Sons: Chichester, UK, 2007.
- Nazzal, A.I.; Street, G.B. Pyrrole styrene graft-copolymers. J. Chem. Soc. Chem. Commun 1985, 6, 375–376.
- Wei, Y.; Hariharan, R.; Patel, S.A. Chemical and electrochemical copolymerization of aniline with alkyl ring-substituted anilines. Macromolecules 1990, 23, 758–764, doi:10.1021/ma00205a011.
- Carrasco, J.; Figueras, A.; Otero, T.F.; Brillas, E. Anodic electrosynthesis and cathodic electrodissolution of poly(2,5-di-(2-thienyl)pyrrole). A new way of processibility. Synth. Met 1993, 61, 253–258, doi:10.1016/0379-6779(93)91270-C.
- Gumbs, R.W. Polythiophene and polypyrrole copolymers. In Handbook of Organic Conductive Molecules and Polymers, 2nd ed.; Nalwa, H.S., Ed.; John Wiley & Sons: Chichester, UK, 1997; pp. 469–504.
- Ferraris, J.P.; Guerrero, D.J. Recent advances in heteroatomic copolymers. In Handbook of Conducting Polymers; Skotheim, T., Elsenbaumer, R.L., Reynolds, J.R., Eds.; Marcel Dekker: New York, NY, USA, 1997; pp. 259–276.
- Otero, T.F.; Vázquez, M.V. Electrogeneration of a composite polypyrrole-carboxymethylcellulose: kinetic study. J. Electroanal. Chem 1995, 397, 171–176, doi:10.1016/0022-0728(95)04168-4.
- Otero, T.F.; Olazábal, V. Electrogeneration of polypyrrole in presence of polyvinylsulphonate. Kinetic study. Electrochim. Acta 1996, 41, 213–220, doi:10.1016/0013-4686(95)00308-2.
- Otero, T.F.; González-Tejera, M.J. Polypyrrole + polyacrylate composites: electrogeneration. J. Electroanal. Chem 1996, 410, 69–77, doi:10.1016/0022-0728(96)04531-7.
- Otero, T.F.; Sansiñena, J.M. Influence of synthesis conditions on polypyrrole-poly(styrenesulphonate) composite electroactivity. J. Electroanal. Chem 1996, 412, 109–116, doi:10.1016/0022-0728(96)04615-3.
- Gómez-Romero, P.; Lira-Cantú, M. Hybrid organic-inorganic electrodes: the molecular material formed between polypyrrole and the phosphomolybdate anion. Adv. Mater 1997, 9, 144–147, doi:10.1002/adma.19970090210.
- Saunders, R.; Murray, K.S.; Flemming, R.J.; Cervini, R.; Allen, N. S. Handbook of Organic Conductive Molecules and Polymers, 3rd ed.; Nalwa, H.S., Ed.; John Wiley & Sons: Chichester, UK, 1997; pp. 634–676.
- Clemente-Leon, M.; Coronado, E.; Galan-Mascaros, J.R.; Gimenez-Saiz, C.; Gomez-Garcia, C.J.; Fernandez-Otero, T. Hybrid molecular materials based on organic molecules and the inorganic magnetic cluster [M-4(H2O)(2)(PW9O34)(2)](10-) (M2+ = Co, Mn). J. Mater. Chem 1998, 8, 309–312, doi:10.1039/a706864f.
- Otero, T.F.; Herrasti, P.; Ocon, P.; Alves, C.R. Electrogeneration of polypyrrole-carboxymethylcellulose composites: electrochemical, microgravimetric and morphological studies. Electrochim. Acta 1998, 43, 1089–1100, doi:10.1016/S0013-4686(97)00216-8.
- Ruckenstein, E.; Chen, J.H. Polypyrrole conductive composites prepared by coprecipitation. Polymer 1991, 32, 1230–1235, doi:10.1016/0032-3861(91)90226-9.
- De Paoli, M.A. Conductive polymer blends and composites. In Handbook of Organic Conductive Molecules and Polymers, 2nd ed.; Nalwa, H.S., Ed.; John Wiley & Sons: Chichester, UK, 1997; pp. 773–798.
- Huang, J.C. Carbon black filled conducting polymers and polymer blends. Adv. Polym. Technol 2002, 21, 299–313, doi:10.1002/adv.10025.
- Otero, T.F.; GonzalezTejera, M.J. Polypyrrole plus polyacrylate composites, kinetic study. J. Electroanal. Chem 1997, 429, 19–25, doi:10.1016/S0022-0728(97)00148-4.
- Otero, T.F. Artificial muscles, electrodissolution and redox processes in conducting polymers. In Handbook of Organic Conductive Molecules and Polymers; Nalwa, H.S., Ed.; John Wiley & Sons: New York, NY, USA, 1997; pp. 517–594.
- Otero, T.F. Electrochemomechanical devices: artificial muscles based on conducting polymers. In Handbook of Conducting Polymers, 3rd ed.; Skotheim, T.A., Elsenhaumer, R.L., Reynolds, J.R., Eds.; Marcel Dekker Inc: New York, NY, USA, 1998; pp. 1015–1028.
- Inzelt, G.; Horányi, G.; Chambers, J.Q. Radiotracer study of the sorption of counter- and co-ions in tetracyanoquinodimethane and poly(vinyl ferrocene) modified electrodes. Electrochim. Acta 1987, 32, 757–763, doi:10.1016/0013-4686(87)85106-X.
- Tsai, E.W.; Pajkossy, T.; Rajeshwar, K.; Reynolds, J.R. Anion-exchange behavior of polypyrrole membranes. J. Phys. Chem 1988, 92, 3560–3565, doi:10.1021/j100323a047.
- Shimidzu, T.; Ohtani, A.; Iyoda, T.; Honda, K. Effective adsorption desorption of cations on a polypyrrole polymer anion composite electrode. J. Chem. Soc. Chem. Commun 1986, 18, 1415–1417.
- Shimidzu, T.; Ohtani, A.; Iyoda, T.; Honda, K. Charge-controllable polypyrrole polyelectrolyte composite membranes. II. Effect of incorporated anion size on the electrochemical oxidation reduction process. J. Electroanal. Chem 1987, 224, 123–135, doi:10.1016/0022-0728(87)85088-X.
- Li, F.B.; Albery, W.J. Electrochemical and in situ electron-paramagnetic resonance studies of polypyrrole doped with polystyrene sulfonate. J. Chem. Soc. Faraday Trans. I 1991, 87, 2949–2954, doi:10.1039/ft9918702949.
- Yue, J.; Wang, Z.H.; Cromack, K.R.; Epstein, A.J.; Macdiarmid, A.G. Effect of sulfonic-acid group on polyaniline backbone. J. Am. Chem. Soc 1991, 113, 2665–2671, doi:10.1021/ja00007a046.
- Otero, T.F.; Santos, F. Polythiophene oxidation: rate coefficients, activation energy and conformational energies. Electrochim. Acta 2008, 53, 3166–3174, doi:10.1016/j.electacta.2007.10.072.
- Otero, T.F.; Abadias, R. Potentiostatic oxidation of poly(3-methylthiophene): influence of the prepolarization time at cathodic potentials on the kinetics. J. Electroanal. Chem 2008, 618, 39–44, doi:10.1016/j.jelechem.2008.02.019.
- Hillman, A.R.; Loveday, D.C.; Swann, M.J.; Eales, R.M.; Hamnett, A.; Higgins, S.J.; Bruckenstein, S.; Wilde, C.P. Charge transport in electroactive polymer-films. Faraday Discuss. Chem. Soc 1989, 88, 151–163, doi:10.1039/dc9898800151.
- Inzelt, G. Mechanism of charge transport in polymer-modified electrodes. In Electroanalytical Chemistry: A Series of Advances; Bard, A.J., Ed.; Marcel Dekker: New York, NY, USA, 1994; pp. 89–243.
- Inzelt, G. Redox Transformations and Transport Processes. In Conducting Polymers; Scholz, F., Ed.; Springer-Verlag: Berlin: Heidelberg, Germany, 2008; pp. 169–224.
- Kiefer, R.; Chu, S.Y.; Kilmartin, P.A.; Bowmaker, G.A.; Cooney, R.P.; Travas-Sejdic, J. Mixed-ion linear actuation behaviour of polypyrrole. Electrochim. Acta 2007, 52, 2386–2391, doi:10.1016/j.electacta.2006.08.058.
- Fermín, D.J.; Teruel, H.; Scharifker, B.R. Changes in the population of neutral species and charge carriers during electrochemical oxidation of polypyrrole. J. Electroanal. Chem 1996, 401, 207–214, doi:10.1016/0022-0728(95)04284-9.
- Sadki, S.; Schottland, P.; Brodie, N.; Sabouraud, G. The mechanisms of pyrrole electropolymerization. Chem. Soc. Rev 2000, 29, 283–293, doi:10.1039/a807124a.
- Otero, T.F.; Angulo, E.; Rodriguez, J.; Santamaria, C. Electrochemomechanical properties from a bilayer—polypyrrole nonconducting and flexible material artificial muscle. J. Electroanal. Chem 1992, 341, 369–375, doi:10.1016/0022-0728(92)80495-P.
- Okuzaki, H.; Funasaka, K. Electromechanical properties of a humido-sensitive conducting polymer film. Macromolecules 2000, 33, 8307–8311, doi:10.1021/ma0000531.
- Smela, E. Conjugated polymer actuators for biomedical applications. Adv. Mater 2003, 15, 481–494, doi:10.1002/adma.200390113.
- Cortes, M.T.; Moreno, J.C. Artificial muscles based on conducting polymers. E-Polymers 2003, 41, 1–42.
- Kaufman, F.B.; Schroeder, A.H.; Engler, E.M.; Patel, V.V. Polymer-modified electrodes—a new class of electrochromic materials. Appl. Phys. Lett 1980, 36, 422–425, doi:10.1063/1.91524.
- Heuer, H.W.; Wehrmann, R.; Kirchmeyer, S. Electrochromic window based on conducting poly (3,4-ethylenedioxythiophene)poly(styrene sulfonate). Adv. Funct. Mater 2002, 12, 89–94, doi:10.1002/1616-3028(20020201)12:2<89::AID-ADFM89>3.0.CO;2-1.
- Mortimer, R.J.; Dyer, A.L.; Reynolds, J.R. Electrochromic organic and polymeric materials for display applications. Displays 2006, 27, 2–18, doi:10.1016/j.displa.2005.03.003.
- Dyer, A.L.; Reynolds, J.R. Electrochromism of conjugated conducting polymers. In Handbook of Conducting Polymers, 3rd ed.; Skotheim, T.A., Elsenbaumer, R.L., Reynolds, J.R., Eds.; CRC Press: Boca Raton, FL, USA, 2007.
- Seshadri, V.; Padilla, J.; Bircan, H.; Radmard, B.; Draper, R.; Wood, M.; Otero, T.F.; Sotzing, G.A. Optimization, preparation, and electrical short evaluation for 30 cm2 active area dual conjugated polymer electrochromic windows. Org. Electron 2007, 8, 367–381, doi:10.1016/j.orgel.2007.01.004.
- Feldman, B.J.; Burgmayer, P.; Murray, R.W. The Potential Dependence of electrical-conductivity and chemical charge storage of poly(pyrrole) films on electrodes. J. Am. Chem. Soc 1985, 107, 872–878, doi:10.1021/ja00290a024.
- Irvin, J.A.; Irvin, D.J.; Stenger-Smith, J.D. Electroactive polymers for batteries and supercapacitors. In Handbook of Conducting Polymers, 3rd ed.; Skotheim, T.A., Elsenbaumer, R.L., Reynolds, J.R., Eds.; CRC Press: Boca Raton, FL, USA, 2007.
- Peng, C.; Zhang, S.W.; Jewell, D.; Chen, G.Z. Carbon nanotube and conducting polymer composites for supercapacitors. Prog. Nat. Sci 2008, 18, 777–788, doi:10.1016/j.pnsc.2008.03.002.
- Burgmayer, P.; Murray, R.W. An ion gate membrane—electrochemical control of ion permeability through a membrane with an embedded electrode. J. Am. Chem. Soc 1982, 104, 6139–6140, doi:10.1021/ja00386a061.
- Ehrenbeck, C.; Juttner, K. Development of an anion cation permeable free-standing membrane based on electrochemical switching of polypyrrole. Electrochim. Acta 1996, 41, 511–518, doi:10.1016/0013-4686(95)00337-1.
- Chan, C.; Chang, S.; Naguib, H.E. Development and characterization of polypyrrole bi-layer and tri-layer thin porous films. Smart. Mater. Struct 2009, 18, 104022, doi:10.1088/0964-1726/18/10/104022.
- Zinger, B.; Miller, L.L. Timed release of chemicals from polypyrrole films. J. Am. Chem. Soc 1984, 106, 6861–6863, doi:10.1021/ja00334a076.
- Miller, L.L.; Zinger, B.; Zhou, Q.X. Electrically controlled release of hexacyanoferrate(4-) from polypyrrole. J. Am. Chem. Soc 1987, 109, 2267–2272, doi:10.1021/ja00242a006.
- Zhong, Y.; Bellamkonda, R.V. Controlled release of anti-inflammatory agent [alpha]-MSH from neural implants. J. Controlled Release 2005, 106, 309–318, doi:10.1016/j.jconrel.2005.05.012.
- Otero, T.F. Biomimetics, artificial muSCLES & NANO-BIO 2007: scientists meet doctors. J. Phys. Conf. Ser 2008, 127, 011001, doi:10.1088/1742-6596/127/1/011001.
- Binh, T.T.N. Development of a biomimetic nanoporous membrane for the selective transport of charged proteins. Bioinspir. Biomim 2008, 3, 035008, doi:10.1088/1748-3182/3/3/035008. 18667763
- Otero, T.F. Soft, wet, and reactive polymers. Sensing artificial muscles and conformational energy. J. Mater. Chem 2009, 19, 681–689, doi:10.1039/b809485c.
- Li, C.; Bai, H.; Shi, G.Q. Conducting polymer nanomaterials: electrosynthesis and applications. Chem. Soc. Rev 2009, 38, 2397–2409, doi:10.1039/b816681c. 19623357
- Otero, T.F. Electro-chemo-mechanical actuators touching and sensing both, physical and chemical ambient. Adv. Sci. Tech 2008, 61, 112–121, doi:10.4028/www.scientific.net/AST.61.112.
- Sansiñena, J.M. Músculos artificiales: dispositivos electroquimiomecánicos basados en polímeros conductores. University of the Basque Country (UPV/EHU): San Sebastian, Spain, 1998.
- Otero, T.F.; Sansiñena, J.M. Artificial muscles based on conducting polymers. Bioelectroch. Bioener 1995, 38, 411–414, doi:10.1016/0302-4598(95)01802-L.
- Otero, T.F.; Cortes, M.T. A sensing muscle. Sens. Actuators B 2003, 96, 152–156, doi:10.1016/S0925-4005(03)00518-5.
- Otero, T.F. Sensing muscles based on conducting polymers: conformational energy. Proceedings of Actuator 08, Bremen, Germany; 2008; pp. 248–251.
- Shimoda, S.; Smela, E. The effect of pH on polymerization and volume change in PPy(DBS). Electrochim. Acta 1998, 44, 219–238, doi:10.1016/S0013-4686(98)00048-6.
- Maw, S.; Smela, E.; Yoshida, K.; Sommer-Larsen, P.; Stein, R.B. The effects of varying deposition current density on bending behaviour in PPy(DBS)-actuated bending beams. Sens. Actuators A 2001, 89, 175–184, doi:10.1016/S0924-4247(00)00512-4.
- Takashima, W.; Pandey, S.S.; Kaneto, K. Cyclic voltammetric and electrochemomechanical characteristics of freestanding polypyrrole films in diluted media. Thin Solid Films 2003, 438–439, 339–345.
- Otero, T.F.; Ariza, M.J. Revisiting the electrochemical and polymeric behavior of a polypyrrole free-standing electrode in aqueous solution. J. Phys. Chem. B 2003, 107, 13954–13961, doi:10.1021/jp0362842.
- John, M.H.; Ian, W.H.; John, B. A comparative analysis of actuator technologies for robotics. In The Robotics Review, 2nd ed. ed.; MIT Press: Cambridge, MA, USA, 1992; pp. 299–342.
- Madden, J.D.W.; Vandesteeg, N.A.; Anquetil, P.A.; Madden, P.G.A.; Takshi, A.; Pytel, R.Z.; Lafontaine, S.R.; Wieringa, P.A.; Hunter, I.W. Artificial muscle technology: physical principles and naval prospects. IEEE J. Oceanic. Eng 2004, 29, 706–728, doi:10.1109/JOE.2004.833135.
- Dunn-Rankin, D.; Leal, E.M.; Walther, D.C. Personal power systems. Progt. Energ. Combust 2005, 31, 422–465, doi:10.1016/j.pecs.2005.04.001.
- Katchalsky, A. Rapid swelling and deswelling of reversible gels of polymeric acids by ionization. Experientia 1949, 5, 319–320, doi:10.1007/BF02172636. 18138361
- Katchalsky, A.; Eisenberg, H. Polyvinylphosphate contractile systems. Nature 1950, 166, 267–267. 15439276
- Kuhn, W.; Hargitay, B.; Katchalsky, A.; Eisenberg, H. Reversible dilation and contraction by changing the state of ionization of high-polymer acid networks. Nature 1950, 165, 514–516, doi:10.1038/165514a0.
- Katchalsky, A.; Zwick, M. Mechanochemistry and ion exchange. J. Polym. Sci 1955, 16, 221–234, doi:10.1002/pol.1955.120168212.
- Pei, Q. B.; Inganas, O. Conjugated polymers and the bending cantilever method—electrical muscles and smart devices. Adv. Mater 1992, 4, 277–278, doi:10.1002/adma.19920040406.
- Otero, T.F.; Angulo, E.; Rodriguez, J.; Santamaria, C. Dispositivos laminares que emplean polímeros conductores capaces de provocar movimientos mecánicosSpanish patent 1992/1/17.
- Otero, T.F.; Rodriguez, J.; Santamaria, C. Músculos artificiales formados por multicapas: polímeros conductores-no conductoresSpanish patent 1992/12/28.
- Mazzoldi, A.; Degl'Innocenti, C.; Michelucci, M.; De Rossi, D. Actuative properties of polyaniline fibers under electrochemical stimulation. Mat. Sci. Eng. C-Bio 1998, 6, 65–72, doi:10.1016/S0928-4931(98)00036-8.
- Madden, J.; Hunter, I.W.; Gilbert, R.J. Development of an artificial muscle fiber composed of the conducting polymer actuator polypyrrole. Gastroenterology 2002, 122, A164.
- Ding, J.; Liu, L.; Spinks, G.M.; Zhou, D.; Wallace, G.G.; Gillespie, J. High performance conducting polymer actuators utilising a tubular geometry and helical wire interconnects. Synth. Met 2003, 138, 391–398, doi:10.1016/S0379-6779(02)00453-8.
- Yamato, K.; Kaneto, K. Tubular linear actuators using conducting polymer, polypyrrole. Anal. Chim. Acta 2006, 568, 133–137, doi:10.1016/j.aca.2005.12.030. 17761253
- Foroughi, J.; Spinks, G.M.; Wallace, G.G. Effect of synthesis conditions on the properties of wet spun polypyrrole fibres. Synth. Met 2009, 159, 1837–1843, doi:10.1016/j.synthmet.2009.06.006.
- Spinks, G.M.; Zhou, D.Z.; Liu, L.; Wallace, G.G. The amounts per cycle of polypyrrole electromechanical actuators. Smart. Mater. Struct 2003, 12, 468–472, doi:10.1088/0964-1726/12/3/318.
- Hara, S.; Zama, T.; Sewa, S.; Takashima, W.; Kaneto, K. Polypyrrole-metal coil composites as fibrous artificial muscles. Chem. Lett 2003, 32, 800–801, doi:10.1246/cl.2003.800.
- Hara, S.; Zama, T.; Ametani, A.; Takashima, W.; Kaneto, K. Enhancement in electrochemical strain of a polypyrrole-metal composite film actuator. J. Mater. Chem 2004, 14, 2724–2725, doi:10.1039/b409169h.
- Hara, S.; Zama, T.; Takashima, W.; Kaneto, K. Polypyrrole-metal coil composite actuators as artificial muscle fibres. Synth. Met 2004, 146, 47–55, doi:10.1016/j.synthmet.2004.06.021.
- Bay, L.; West, K.; Sommer-Larsen, P.; Skaarup, S.; Benslimane, M. A conducting polymer artificial muscle with 12% linear strain. Adv. Mater 2003, 15, 310–313, doi:10.1002/adma.200390075.
- Lu, W.; Fadeev, A.G.; Qi, B.H.; Smela, E.; Mattes, B.R.; Ding, J.; Spinks, G.M.; Mazurkiewicz, J.; Zhou, D.Z.; Wallace, G.G.; MacFarlane, D.R.; Forsyth, S.A.; Forsyth, M. Use of ionic liquids for pi-conjugated polymer electrochemical devices. Science 2002, 297, 983–987, doi:10.1126/science.1072651. 12098704
- Okuzaki, H. A biomorphic origami actuator fabricated by folding a conducting paper. J. Phys. Conf. Ser 2008, 127, 012001, doi:10.1088/1742-6596/127/1/012001.
- Kaneto, K.; Sonoda, Y.; Takashima, W. Direct measurement and mechanism of electro-chemomechanical expansion and contraction in polypyrrole films. Jpn. J. Appl. Phys. 2000, 5918–5922, doi:10.1143/JJAP.39.5918.
- Pandey, S.S.; Takashima, W.; Kaneto, K. Structure property correlation: electrochemomechanical deformation in polypyrrole films. Thin Solid Films 2003, 438, 206–211, doi:10.1016/S0040-6090(03)00754-5.
- Zama, T.; Hara, S.; Takashima, W.; Kaneto, K. The correlation between electrically induced stress and mechanical tensile strength of polypyrrole actuators. Bull. Chem. Soc. Jpn 2004, 77, 1425–1426, doi:10.1246/bcsj.77.1425.
- Baughman, R.H.; Shacklette, L.W. Application of dopant-induced structure-property changes of conducting polymers. In Science and Application of Conducting Polymers; Salaneck, W.R., Clark, D.T., Samuelsen, E.J., Eds.; IOP Publishing Ltd: Bristol, UK, 1991; pp. 47–61.
- Pei, Q.B.; Inganas, O. Electrochemical applications of the bending beam method. I. Mass-transport and volume changes in polypyrrole during redox. J. Phys. Chem 1992, 96, 10507–10514, doi:10.1021/j100204a071.
- Suarez, M.F.; Compton, R.G. In situ atomic force microscopy study of polypyrrole synthesis and the volume changes induced by oxidation and reduction of the polymer. J. Electroanal. Chem 1999, 462, 211–221, doi:10.1016/S0022-0728(98)00414-8.
- Smela, E.; Gadegaard, N. Surprising volume change in PPy(DBS): an atomic force microscopy study. Adv. Mater 1999, 11, 953–957, doi:10.1002/(SICI)1521-4095(199908)11:11<953::AID-ADMA953>3.0.CO;2-H.
- Smela, E.; Gadegaard, N. Volume change in polypyrrole studied by atomic force microscopy. J. Phys. Chem. B 2001, 105, 9395–9405, doi:10.1021/jp004126u.
- Barbero, C.; Kotz, R. Nanoscale Dimensional changes and optical-properties of polyaniline measured by in-situ spectroscopic ellipsometry. J. Electrochem. Soc 1994, 141, 859–865, doi:10.1149/1.2054847.
- Ehrenbeck, C.; Juttner, K. Ion conductivity and permselectivity measurements of polypyrrole membranes at variable states of oxidation. Electrochim. Acta 1996, 41, 1815–1823, doi:10.1016/0013-4686(95)00500-5.
- Juttner, K.; Ehrenbeck, C. Electrochemical measurements of the ion conductivity, permselectivity and transference numbers of polypyrrole and polypyrrole derivatives. J. Solid State Electrochem 1998, 2, 60–66, doi:10.1007/s100080050065.
- Andrade, E. M.; Molina, F.V.; Florit, M.I.; Posadas, D. Volume changes of poly(2-methylaniline) upon redox switching—anion and relaxation effects. Electrochem. Solid-State Lett 2000, 3, 504–507.
- Lizarraga, L.; Andrade, E.M.; Molina, F.V. Swelling and volume changes of polyaniline upon redox switching. J. Electroanal. Chem 2004, 561, 127–135, doi:10.1016/j.jelechem.2003.07.026.
- Davis, A.P. Nanotechnology—synthetic molecular motors. Nature 1999, 401, 120–121. 10490015
- Kay, E.R.; Leigh, D.A.; Zerbetto, F. Synthetic molecular motors and mechanical machines. Angew. Chem. Int. Edit 2007, 46, 72–191, doi:10.1002/anie.200504313.
- Pei, Q.; Inganäs, O. Electrochemical muscles: bending strips built from conjugated polymers. Synth. Met 1993, 57, 3718–3723, doi:10.1016/0379-6779(93)90503-O.
- Takashima, W.; Kaneko, M.; Kaneto, K.; Macdiarmid, A.G. The electrochemical actuator using electrochemically-deposited poly-aniline film. Synth. Met 1995, 71, 2265–2266, doi:10.1016/0379-6779(94)03252-2.
- Smela, E.; Inganäs, O.; Pei, Q.B.; Lundstrom, I. Electrochemical muscles—micromachining fingers and corkscrews. Adv. Mater 1993, 5, 630–632, doi:10.1002/adma.19930050905.
- Jager, E.W.H.; Smela, E.; Inganäs, O. Microfabricating conjugated polymer actuators. Science 2000, 290, 1540–1545, doi:10.1126/science.290.5496.1540. 11090345
- Jager, E.W.H.; Inganäs, O.; Lundstrom, I. Microrobots for micrometer-size objects in aqueous media: Potential tools for single-cell manipulation. Science 2000, 288, 2335–2338, doi:10.1126/science.288.5475.2335. 10875911
- Baughman, R.H. Conducting polymer artificial muscles. Synth. Met 1996, 78, 339–353, doi:10.1016/0379-6779(96)80158-5.
- Takashima, W.; Pandey, S.S.; Kaneto, K. Investigation of bi-ionic contribution for the enhancement of bending actuation in polypyrrole film. Sens. Actuators B 2003, 89, 48–52, doi:10.1016/S0925-4005(02)00426-4.
- Han, G.; Shi, G. Conducting polymer electrochemical actuator made of high-strength three-layered composite films of polythiophene and polypyrrole. Sensor Actuat. B-Chem 2004, 99, 525–531, doi:10.1016/j.snb.2004.01.001.
- Higgins, S.J.; Lovell, K.V.; Rajapakse, R.M.G.; Walsby, N.M. Grafting and electrochemical characterisation of poly-(3,4-ethylenedioxythiophene) films, on Nafion and on radiation-grafted polystyrenesulfonate-polyvinylidene fluoride composite surfaces. J. Mater. Chem 2003, 13, 2485–2489, doi:10.1039/b303424k.
- Deshpande, S.D.; Kim, J.; Yun, S.R. New electro-active paper actuator using conducting polypyrrole: actuation behaviour in LiClO4 acetonitrile solution. Synth. Met 2005, 149, 53–58, doi:10.1016/j.synthmet.2004.11.001.
- Blonsky, P. M.; Meridian, I. Structurally stable gelled electrolytes. 1997.
- Song, M.K.; Cho, J.Y.; Cho, B.W.; Rhee, H.W. Characterization of UV-cured gel polymer electrolytes for rechargeable lithium batteries. J. Power Sources 2002, 110, 209–215, doi:10.1016/S0378-7753(02)00258-6.
- Vidal, F.; Popp, J.F.; Plesse, C.; Chevrot, C.; Teyssie, D. Feasibility of conducting semi-interpenetrating networks based on a poly(ethylene oxide) network and poly(3,4-ethylenedioxythiophene) in actuator design. J. Appl. Polym. Sci 2003, 90, 3569–3577, doi:10.1002/app.13055.
- Plesse, C.; Vidal, F.; Randriamahazaka, H.; Teyssie, D.; Chevrot, C. Synthesis and characterization of conducting interpenetrating polymer networks for new actuators. Polymer 2005, 46, 7771–7778, doi:10.1016/j.polymer.2005.03.103.
- Plesse, C.; Vidal, F.; Gauthier, C.; Pelletier, J.M.; Chevrot, C.; Teyssié, D. Poly(ethylene oxide)/polybutadiene based IPNs synthesis and characterization. Polymer 2007, 48, 696–703, doi:10.1016/j.polymer.2006.11.053.
- Cho, M.; Seo, H.; Nam, J.; Choi, H.; Koo, J.; Lee, Y. High ionic conductivity and mechanical strength of solid polymer electrolytes based on NBR/ionic liquid and its application to an electrochemical actuator. Sensor Actuat. B-Chem 2007, 128, 70–74, doi:10.1016/j.snb.2007.05.032.
- Tran-Van, F.; Beouch, L.; Vidal, F.; Yammine, P.; Teyssie, D.; Chevrot, C. Self-supported semi-interpenetrating polymer networks for new design of electrochromic devices. Electrochim. Acta 2008, 53, 4336–4343, doi:10.1016/j.electacta.2007.12.087.
- Vidal, F.; Plesse, C.; Palaprat, G.; Juger, J.; Citerin, J.; Kheddar, A.; Chevrot, C.; Teyssie, D. Synthesis and characterization of ipns for electrochemical actuators. In Artificial Muscle Actuators Using Electroactive Polymers; Vincenzini, P., BarCohen, Y., Carpi, F., Eds.; Trans Tech Publications Ltd: Stafa-Zurich, Switzerland, 2009; pp. 8–17.
- Otero, T.F.; Cortes, M.T.; Boyano, I. Macroscopic devices and complex movements developed with artificial muscles. In Smart Structures and Materials 2002: Electroactive Polymer Actuators and Devices (Eapad); Bellingham, WA, USA, 2002; pp. 395–402.
- Otero, T.F.; Cortes, M.T.; Arenas, G.V. Linear movements from two bending triple-layers. Electrochim. Acta 2007, 53, 1252–1258, doi:10.1016/j.electacta.2007.01.081.
- Otero, T.F.; Broschart, M. Polypyrrole artificial muscles: a new rhombic element. Construction and electrochemomechanical characterization. J. Appl. Electrochem 2006, 36, 205–214, doi:10.1007/s10800-005-9048-0.
- Vozzi, G.; Carpi, F.; Mazzoldi, A. Realization of conducting polymer actuators using a controlled volume microsyringe system. Smart. Mater. Struct 2006, 15, 279–287, doi:10.1088/0964-1726/15/2/006.
- Alici, G.; Huynh, N. N. Performance quantification of conducting polymer actuators for real applications: a microgripping system. IEEE ASME Trans. Mechatronics 2007, 12, 73–84, doi:10.1109/TMECH.2006.886256.
- Smela, E.; Inganäs, O.; Lundstrom, I. Controlled folding of micrometer-size structures. Science 1995, 268, 1735–1738, doi:10.1126/science.268.5218.1735. 17834992
- Pede, D.; Smela, E.; Johansson, T.; Johansson, M.; Inganäs, O. A general-purpose conjugated-polymer device array for imaging. Adv. Mater 1998, 10, 233–237, doi:10.1002/(SICI)1521-4095(199802)10:3<233::AID-ADMA233>3.0.CO;2-M.
- Smela, E.; Kallenbach, M.; Holdenried, J. Electrochemically driven polypyrrole bilayers for moving and positioning bulk micromachined silicon plates. J. Microelectromech. S 1999, 8, 373–383, doi:10.1109/84.809051.
- Smela, E. A microfabricated movable electrochromic “pixel” based on polypyrrole. Adv. Mater 1999, 11, 1343–1345, doi:10.1002/(SICI)1521-4095(199911)11:16<1343::AID-ADMA1343>3.0.CO;2-V.
- Jager, E.W.H.; Smela, E.; Inganäs, O.; Lundstrom, I. Polypyrrole microactuators. Synth. Met 1999, 102, 1309–1310, doi:10.1016/S0379-6779(98)01000-5.
- Jager, E.W.H.; Inganäs, O.; Lundstrom, I. Perpendicular actuation with individually controlled polymer microactuators. Adv. Mater 2001, 13, 76–79, doi:10.1002/1521-4095(200101)13:1<76::AID-ADMA76>3.0.CO;2-I.
- Roemer, M.; Kurzenknabe, T.; Oesterschulze, E.; Nicoloso, N. Microactuators based on conducting polymers. Anal. Bioanal. Chem 2002, 373, 754–757, doi:10.1007/s00216-002-1414-8. 12194034
- He, X.M.; Li, C.; Chen, F.G.; Shi, G.Q. Polypyrrole microtubule actuators for seizing and transferring microparticles. Adv. Funct. Mater 2007, 17, 2911–2917, doi:10.1002/adfm.200600869.
- Kiefer, R.; Mandviwalla, X.; Archer, R.; Tjahyono, S.S.; Wang, H.; MacDonald, B.; Bowmaker, G.A.; Kilmartin, P.A.; Travas-Sejdic, J. The application of polypyrrole trilayer actuators in microfluidics and robotics—art. no. 69271E. In Electroactive Polymer Actuators and Devices (Eapad) 2008; Bellingham, WA, USA, 2008; pp. E9271–E9271.
- Otero, T.F.; Cortes, M.T. Artificial muscle: movement and position control. Chem. Commun 2004, 3, 284–285.
- Otero, T.F.; Sansinena, J.M. Bilayer dimensions and movement in artificial muscles. Bioelectroch. Bioener 1997, 42, 117–122, doi:10.1016/S0302-4598(96)05112-4.
- Otero, T.F.; Sansinena, J.M. Soft and wet conducting polymers for artificial muscles. Adv. Mater 1998, 10, 491–494, doi:10.1002/(SICI)1521-4095(199804)10:6<491::AID-ADMA491>3.0.CO;2-Q. 21647986
- Otero, T.F.; Cortes, M.T. Electrochemical characterization and control triple-layer muscles. In Smart Structures and Materials 2000: Electroactive Polymer Actuators and Devices (Eapad); Bellingham, WA, USA, 2000; pp. 252–260.
- Otero, T.F.; Cortes, M.T. Characterization of triple layers. In Smart Structures and Materials 2001: Electroactive Polymer Actuators and Devices; Bellingham, WA, USA, 2001; pp. 93–100.
- Otero, T.F.; Boyano, I.; Cortes, M.T.; Vazquez, G. Nucleation, non-stoiquiometry and sensing muscles from conducting polymers. Electrochim. Acta 2004, 49, 3719–3726, doi:10.1016/j.electacta.2004.01.085.
- Otero, T.F.; Cortes, M.T. Artificial muscles with tactile sensitivity. Adv. Mater 2003, 15, 279–282, doi:10.1002/adma.200390066.
- Otero, T.F.; Cortes, M.T.; Boyano, L.; Vazquez, G. Nucleation, non-stoiquiometry, and tactile muscles with conducting polymers. In Smart Structures and Materials 2004: Electroactive Polymer Actuators and Devices (Eapad); Bellingham, WA, USA, 2004; pp. 425–432.
|Table 1. Electrochemical properties of conducting polymers, related functions and minded biological organs.|
|Electrochemomechanical||Change of volume||Muscles|
|Electrochromic||Change of color||Mimetic skins|
|Charge storage||Current generation||Electric organs|
|Electroporosity||Transversal ionic flow||Membrane|
|Chemical or pharmacological storage||Chemical modulation or chemical dosage||Glands|
|Electron/ion transduction||ΔV (Chem/Phys. properties)||Bio-sensors|
|Electron/neurotransmitter||Channel V action||Nervous interface|
© 2010 by the authors; licensee Molecular Diversity Preservation International, Basel, Switzerland. This article is an open-access article distributed under the terms and conditions of the Creative Commons Attribution license (http://creativecommons.org/licenses/by/3.0/).